bacillus spores as building blocks for stimuli-responsive ...· bacillus spores as building blocks
Post on 28-Jun-2018
Embed Size (px)
Bacillus spores as building blocks for stimuli-responsive materials and nanogeneratorsXi Chen1, L. Mahadevan2,3,4, Adam Driks5 and Ozgur Sahin1,4*
Materials that respond mechanically to external chemicalstimuli have applications in biomedical devices, adaptive archi-tectural systems, robotics and energy harvesting15. Inspired bybiological systems, stimuli-responsive materials have beencreated that can oscillate2, transport fluid3, provide homeosta-sis4 and undergo complex changes in shape5. However, theeffectiveness of synthetic stimuli-responsive materials in gen-erating work is limited when compared with mechanical actua-tors6. Here, we show that the mechanical response of Bacillusspores to water gradients exhibits an energy density of morethan 10 MJ m23, which is two orders of magnitude higherthan synthetic water-responsive materials7,8. We also identifiedmutations that can approximately double the energy density ofthe spores and found that they can self-assemble into dense,submicrometre-thick monolayers on substrates such as siliconmicrocantilevers and elastomer sheets, creating bio-hybridhygromorph actuators9,10. To illustrate the potential appli-cations of the spores, we used them to build an energy-harvest-ing device that can remotely generate electrical power from anevaporating body of water.
In plants and many other biological organisms, water-responsivestructures accomplish vital tasks such as the ascent of sap and thedispersal and self-burial of seeds1115. Because of their critical func-tions, these water-responsive structures could possibly exhibit highenergy densities and therefore potentially serve as the buildingblocks for stimuli-responsive materials that are efficient energyconverters and actuators. In this work, we investigated the potentialof Bacillus spores to convert energy from water gradients andto serve as the building blocks for high-energy-density stimuli-responsive materials.
Bacillus spores are dormant cells that can withstand harshenvironmental conditions for long periods of time and still maintainbiological functionality16 (Fig. 1a,b). Despite their dormancy, sporesare dynamic structures. For example, Bacillus spores respond tochanges in relative humidity by expanding and shrinking, changingtheir diameter by as much as 12% (refs 1720). We used an atomicforce microscope (AFM)-based experiment (Fig. 1c) to determinethe energy density of individual spores as they respond to changesin relative humidity. By adjusting the force and relative humidity,we created a thermodynamic cycle in which individual spores passthrough four stages (Fig. 1d). In stage I, the spores rest at low relativehumidity (20%). In stage II, the cantilever exerts a predeterminedforce (loading). In stage III, the spores are subjected to high relativehumidity (90%). Finally, in stage IV, the force is reduced back tozero. The cycle is completed on lowering the relative humidity.
Figure 1e presents experimentally measured force versus heightcurves as spores of two species (Bacillus subtilis and Bacillus thuringiensis)
and of a B. subtilis strain bearing mutations in cotE and gerE(B. subtilis cotE gerE)21 proceed through the thermodynamiccycle. The areas enclosed by the force versus height curves inFig. 1e correspond to the amount of work done by the spores (onthe order of 1 pJ). To estimate the energy density of the spores, itis necessary to determine the volume of the material contributingto work. However, because stresses are localized near the apex ofthe AFM tip, it is difficult to define the interaction volume. Toaccount for the non-uniformity in stress and strain distributions,we approximated the spore geometry as a cylindrical object(diameter length of 0.7 1.5 mm) indented by a sphericaltip (radius of 0.85 mm). We estimated the spore energy densityby comparing the energy of indentation calculated for this geometrywith a case in which the spore is uniformly compressed by a planarindenter with the same depth of indentation (see SupplementarySection 1 for details of the calculations; note that the spore dia-meters used in these calculations are based on values determinedexperimentally with AFM height measurements). The resulting esti-mates of the energy densities and their standard deviations areplotted in Fig. 1f together with the maximum strains correspondingto the relative changes in spore diameter.
We note that the spores studied here showed differences in bothenergy densities and strain responses. In particular, the differencesin energy densities between B. subtilis (10.6 MJ m23) and theother two spores (B. subtilis cotE gerE, 19.2 MJ m23; B. thuringiensis,21.3 MJ m23) are statistically significant (mean values are separatedby more than four standard deviations). These differences can bepartially explained by the relative size and swelling ability of thecortex layers in each species. For example, the B. subtilis cotE gerEmutant spore lacks most of its coat layers21, thereby reducing thevolume of the spore contributed by the coat and increasing the rela-tive cortex volume (Fig. 1b). These effects may explain the increasein strain response and energy density due to these mutations. Wealso note that the maximum forces we could reversibly apply tothe spores were consistently higher for cotE gerE mutant sporesthan wild-type spores, which also contributed to the relativeincrease in energy density of these mutants. This favourableoutcome suggests that an improved understanding of the hierarch-ical spore ultrastructure under extreme forces22 can facilitate the useof genetic manipulation to allow further increases in energy densityand strain responses. Note that improving the physical character-istics of materials through genetic manipulation has been success-fully utilized in related areas like virus-based electromechanicalconversion and material synthesis23,24, highlighting the distinctadvantage of using biologically based materials.
Because most of the water absorption and release in spores is dueto the cortex, the energy density of the cortex alone is likely to be
1Department of Biological Sciences and Department of Physics, Columbia University, New York, New York 10027, USA, 2School of Engineering and AppliedSciences, Department of Physics, Department of Organismic and Evolutionary Biology, Harvard University, Cambridge, Massachusetts 02138, USA, 3KavliInstitute for Nanobio Science and Technology, Harvard University, Cambridge, Massachusetts 02138, USA, 4Wyss Institute for Biologically InspiredEngineering at Harvard University, Boston, Massachusetts 02115, USA, 5Department of Microbiology and Immunology, Loyola University Medical Center,2160 S. First Avenue, Maywood, Illinois 60153, USA. *e-mail: email@example.com
LETTERSPUBLISHED ONLINE: 26 JANUARY 2014 | DOI: 10.1038/NNANO.2013.290
NATURE NANOTECHNOLOGY | VOL 9 | FEBRUARY 2014 | www.nature.com/naturenanotechnology 137
2014 Macmillan Publishers Limited. All rights reserved
even higher than that for the entire spore. A simple estimate can bebased on relative cortex volume, which could be obtained byapproximating the coat and cortex layers as cylindrical shells encas-ing the core with respective thicknesses and radius of 60 nm, 60 nmand 200 nm (the numbers are estimated from cross-section trans-mission electron microscopy (TEM) images in ref. 20). Thesenumbers result in a cortex energy density of 3060 MJ m23. Wealso estimate the strain in the cortex to be 50%, assuming thatthe majority of the diameter change is due to expansion of thislayer. Figure 1g compares the estimated energy densities andstrain responses of the spores and the cortex with typical valuesreported for materials frequently used or studied in the context ofactuators and stimuli-responsive materials. As seen in this compari-son, spores are remarkable actuators with extreme characteristics.We speculate that the origin of the high energy density lies in thenanoscale structure and material properties of the spores.Confinement of water in nanoscale pores of the spore cortex maybe preventing water cavitation, which would create large negativepressures in water as a response to dehydration. At the same time,the high elastic modulus of the spores20 may be preventing the col-lapse of the spore structure under large negative pressures, allowingthem to change shape under high pressure.
The mechanical behaviour of individual spores suggests that theycan serve as the building blocks for high-energy-density stimuli-responsive materials. The spores small physical dimensionssuggest that self-assembly may be sufficient to form approximatemonolayers following the deposition and drying of a spore suspen-sion on a substrate (Fig. 2a,b). With this approach, we assembledB. subtilis spores on silicon microcantilevers and latex rubbersheets, and observed their response to changes in water potential.We chose B. subtilis in part because of its lack of an additionalouter layer, the exosporium, as is possessed by some species, andwhich might reduce the packing density25. The differential strainexerted by the spores caused a change in the curvatures of the
microcantilevers and latex sheets, as shown in Fig. 2c,g. These defor-mations allowed us to characterize the response of the single-spore-thick layer to changes in water potential. We determined the curva-ture of the spore-coated latex sheet from images taken by a camera.However, because of the small sizes of the microcantilevers, we usedan AFM to characterize the cantilever deformations by reflecting thelaser from the uncoated surface (Fig. 2d,e).
Measurements with the spore-coated microcantilever demon-strated excellent reversibility and a relatively fast response to vari-ations in water potential. Figure 2f shows the response of themic